1.
Int j simul model 9 (2010) 1, 17-27ISSN 1726-4529 Professional paper FINITE ELEMENT ANALYSIS OF SUPERPLASTIC BLOW-FORMING OF Ti-6Al-4V SHEET INTO CLOSED ELLIP-CYLINDRICAL DIE Chen, D.-C.; Chen, W.-J.; Lin, J.-Y.; Jheng, M.-W. & Chen, J.-M. Department of Industrial Education and Technology, National Changhua University of Education, Changhua 500, Taiwan, R.O.C. E-Mail: dcchen@cc.ncue.edu.twAbstractUtilizing commercial DEFORMTM 3D finite element (FE) software, this study performs aseries of numerical simulations to investigate the superplastic blow-forming of Ti-6Al-4Vtitanium alloy into a closed ellip-cylindrical die. In performing the simulations, it is assumedthat the die is a rigid body and the titanium alloy sheet is a rigid-plastic material withhomogeneous and isotropic properties. The simulations focus specifically on the respectiveeffects of the shear friction factor, the die entry radius, the die height and the die’s short-axislength on the thickness, effective stress, effective strain and critical damage distributionswithin the blow-formed product. Overall, the simulation results confirm the suitability of theDEFORMTM 3D software for modelling the superplastic blow-forming of Ti-6Al-4V titaniumalloy.(Received in March 2009, accepted in September 2009. This paper was with the authors 2 months for 1 revision.)Key Words: Finite Element Analysis, Superplastic Blow-Forming, Titanium Alloy, Ellip-Cylindrical Die1. INTRODUCTIONThe term ’superplasticity’ describes the capability of certain polycrystalline materials such as8090 Al-Li alloy, Ti-6Al-4V alloy, and so forth, to undergo extensive tensile plasticdeformation prior to failure under specific temperature and strain-rate conditions. Thecharacteristics of superplasticity, namely a low flow stress and a large elongation, have led tothe development of a variety of ‘superplastic forming’ (SPF) processes such as forging,extrusion, blow-forming, and so on (Miller and White [1]; Al-Naib and Duncan [2]). Hwanget al. [3-4] utilized commercial DEFORMTM FE software to investigate the pressurizationprofile and sheet thickness distribution of 8090 Al-Li sheets blow-formed into closedellip-cylindrical and rectangular dies. A pressure control algorithm is proposed to keep themaximum stain rate in the deformation zone of the sheet equal to the target value. SenthilKumar et al. [5] investigated the superplastic deformation behaviour of AA7475 aluminiumalloy during its blow-forming into a circular die and compared the results obtained using asimple theoretical model with those generated by ABAQUS FE code. Utilizing MARCsimulation software, Morsy and Manabe [6] confirmed the validity of the materialcharacteristics and stress–strain rate relationship obtained from multi-dome tests, and showedthat the multi-dome test was applicable not only to simple processes such as freebulge-forming, but also to more complex processes such as rectangular box forming. Hwanget al. [7] developed a mathematical model based upon the finite-difference method toinvestigate the plastic deformation behaviour of alloy sheets during blow-forming into aclosed conical die. It was shown that the theoretical predictions for the respective effects ofDOI:10.2507/IJSIMM09(1)2.137 17
2.
Chen, Chen, Lin, Jheng, Chen: Finite Element Analysis of Superplastic Blow-Forming of …the die entry radius, the friction coefficient, and the inclination angle of the die on thepressurization profile, forming time and thickness distribution were in good agreement withthe experimental results. Bonet et al. [8] proposed various pressure control algorithms for FE simulations of SPFprocesses. Kim et al. [9] presented a combined FEA / optimization scheme for predicting theinitial blank thickness distribution required to achieve a uniform final thickness insuperplastic blow-formed products. Huang et al. [10] performed a series of experimental trialsto validate the processing conditions predicted by ABAQUS FE simulations for optimizingthe sheet thickness distribution in superplastic forming processes. Yarlagadda et al. [11]performed FE simulations of the superplastic forming of Al-Ti alloys and used the resultsobtained for the deformed shape, the stress-strain distribution and the thickness evolutionacross the facets of the fully formed surface, respectively, to optimize the processingconditions and to predict the forming time. Hambli et al. [12] presented 2D and 3D finiteelement models for predicting the optimum pressure cycle law, the deformed shape, the strainrate distribution and the thickness evolution during superplastic forming processes. Thevalidity of the pressure prediction algorithm used in the numerical solution procedure wasconfirmed by comparing the numerical results with the experimental observations. Verma and Kim [13] investigated and understand the effect of Cu additions on bothelevated temperature formability and ambient temperature mechanical properties of AA5083alloy. A detailed FE analysis of superplastic gas-blow forming was carried out using amodified microstructure-based constitutive model that accounts for grain growth andcavitation by Nazzal et al. [14]. Wu et al. [15] studied an analysis of cavitation characteristics ofa SP5083 Al alloy through usage of blow forming. Sorgente et al. [16] analyzed the formingbehaviour of a commercial AZ31 Mg alloy sheet at elevated temperature both in free bulgingand in closed die tests. In a previous study (Chen et al., [17-18]), the current group utilized the Taguchi designmethod to identify the processing parameters required to optimize the thickness distribution ofTi-6Al-4V titanium alloy following its superplastic blow-forming into an ellip-cylindrical die,and simulated the superplastic blow-forming of same alloy sheet into triangular, square andconical awl-shaped dies. In the present study, DEFORMTM 3D FE software is used toinvestigate the plastic deformation behaviour of Ti-6Al-4V alloy sheet blow-formed into aclosed ellip-cylindrical die. The simulations focus principally on the respective effects of theshear friction factor, the die entry radius, the die height and the length of the die’s short axison the thickness, effective stress, effective strain and critical damage characteristics of theformed sheet.2. FINITE-ELEMENT FORMULATIONAccording to Kim and Yang [19], the FE formulation for rigid-plastic deformation in amaterial subject to work hardening has the form ∫ w (σ + αΔtε&H )δε&dV + K ∫ w ε&vδε&v dV − ∫ w ( fi + αΔfi )δvi dS = 0 , V V Sf (1)where σ = (3 / 2)σ ij σ ij , ε = ( 2 / 3)ε ij ε ij and ε v = ε ii . Additionally, K, σ ij , H’ and α are & & & & & the penalty constant, the deviatoric stress, the strain-hardening rate and the work-hardeningconstant (0 ≤ α ≤1), respectively, while Vw and Swf are the volume and tractional boundarysurface of the workpiece, respectively. The DEFORMTM 3D FE simulations performed in this study are based on a flowformulation approach using an updated Lagrangian procedure. The nonlinear equations in theFE software are solved using a combined direct iteration method / Newton-Raphson scheme. 18
3.
Chen, Chen, Lin, Jheng, Chen: Finite Element Analysis of Superplastic Blow-Forming of …In the solution procedure, the direct iteration method is used to generate a suitable initialestimate, and the Newton-Raphson method is then applied to obtain a rapid convergence fromthis initial estimate to the final solution. The iterative solution procedure terminates when thefollowing conditions are achieved: a velocity error norm of Δv / v ≤ 0.005 and a force errornorm of ΔF / F ≤ 0.05 , where v is ( v T v)1 / 2 . The deformation behaviour of a superplastic alloy is governed by the relationship betweenthe von Mises equivalent stress and the equivalent strain rate, and is generally expressed asfollows: & σ = Kε ms , (2)where K is the material coefficient, and includes the combined effect of both the equivalentstrain and the grain size; and ms is the strain-rate sensitivity. To express the lubricity at the interface between the ellip-cylindrical die and Ti-6Al-4Valloy sheet, the constant shear friction τs = mk is adopted, where k is the yield shear stress ofthe deforming material, and m is the friction factors (0 ≤ m ≤1). The friction factors mbetween the Ti-6Al-4V alloy sheet and ellip-cylindrical die is determined by the so called ringcompression test.3. RESULTS AND DISCUSSIONIn simulating the superplastic blow-forming of the Ti-6Al-4V alloy sheet, the followingassumptions are made: (1) the ellip-cylindrical die is a rigid body; (2) the titanium alloy sheetis a rigid-plastic material with homogeneous and isotropic properties; and (3) the frictionfactor between the titanium sheet and the ellip-cylindrical die remains constant throughout theblow-forming process. Fig. 1 presents the stress-strain relationship for the Ti-6Al-4V titaniumalloy at a temperature of 1000°C and a strain rate of 0.1 s-1. As shown, the maximum flowstress (~42 MPa) occurs at a strain of 0.5. In performing the present simulations, the initialsheet thickness (t), the long axis of the die (a), the root radius of the die (r), the processingtemperature (T) and the strain rate are all assigned constant values (see Table I). However, asshown in Table II, the values assigned to the short-axis length of the die (b), the die height (h),the die entry radius (R), and the shear friction factor (m) vary from one simulation to the next. 42 41 40 39Flow Stress (MPa) 38 37 36 Temperature (oC) 1000 35 34 33 32 31 0 0.1 0.2 0.3 0.4 0.5 StrainFigure 1: Stress-strain relationship for Ti-6Al-4V alloy (strain rate = 0.1 s-1). 19
4.
Chen, Chen, Lin, Jheng, Chen: Finite Element Analysis of Superplastic Blow-Forming of … Table I: Constant parameters in superplastic blow-forming simulations. Thickness Long axis Die root Temperature Strain Material of sheet (t) of the die (a) radius (r) (T) rate Ti-6Al-4V 1.5 mm 40 mm 2 mm 1000°C 0.1 (1/s) Fig. 2 presents the meshed models of the Ti-6Al-4V alloy sheet and ellip-cylindrical die atsteps 1, 8, 12, 22 and 47 of the simulated blow-forming process. Note that due to the inherentsymmetry of the ellip-cylindrical die, only one-quarter of the sheet / die model (comprising8000 3D elements) is presented here. As shown, in simulating the blow-forming process, thefollowing geometry parameters and experimental conditions were assumed: t (thickness ofsheet) = 1.5 mm, a (long axis of the die) = 40 mm, b (short axis of the die) = 20 mm, R (dieentry radius) = 5 mm, r (die root radius) = 2 mm, h (die height) = 10 mm, m (shear frictionfactor) = 0.5, T (temperature of Ti-6Al-4V alloy sheet) = 1000°C, and strain rate = 0.1 s-1. Inaddition, an assumption was made that the titanium sheet was firmly attached to the peripheryof the die such that no metal flowed from the periphery regions of the sheet into the die cavityduring the forming process. Table II: Variable parameters in superplastic blow-forming simulations. Factors Short axis Die height Die entry Shear friction No. (b) (h) radius (R) factor (m) 1 20 10 5 0.5 2 20 10 5 0.2 3 20 10 5 0.05 4 20 10 7 0.5 5 20 10 7 0.2 6 20 10 7 0.05 7 20 9 5 0.5 8 20 9 5 0.2 9 20 9 5 0.05 10 20 9 7 0.5 11 20 9 7 0.2 12 20 9 7 0.05 13 30 10 5 0.5 14 30 10 5 0.2 15 30 10 5 0.05 16 30 10 7 0.5 17 30 10 7 0.2 18 30 10 7 0.05 19 30 9 5 0.5 20 30 9 5 0.2 21 30 9 5 0.05 20
5.
Chen, Chen, Lin, Jheng, Chen: Finite Element Analysis of Superplastic Blow-Forming of …t = 1.5 mm, a = 40 mm, b = 20 mm, R = 5 mm, r = 2 mm, h = 10 mm, m = 0.5, T = 1000°C,Strain rate = 0.1 s-1 Ellip-cylindrical die Ti-6Al-4V (a) Step 1 h R r (b) Step 8 (c)Step 12 (d) Step 22 (e) Step 47Figure 2: Finite element model of titanium sheet and ellip-cylindrical die. 21
6.
Chen, Chen, Lin, Jheng, Chen: Finite Element Analysis of Superplastic Blow-Forming of … The modelling formulations of various ductility damage values were reported by Klockeet al. [20]. The damage induced in the superplastic blow-forming of the present titanium alloysheet is evaluated using the following normalized C&L criterion: εf σ max ∫ 0 σ dε = C d , (3)where σ max is the maximum ductile stress, ε f is the effective fracture strain, and Cd is thedamage value of the material. Fig. 3 illustrates the distributions of the damage, effective strain and effective stress,respectively, within the titanium alloy sheet following superplastic blow-forming underconditions of: t = 1.5 mm, a = 40 mm, b = 30 mm, R = 5 mm, r = 2 mm, h = 9 mm, m = 0.5, T= 1000°C, and a strain rate of 0.1 s-1. Figs. 3(a) and 3(b) reveal that the maximum damage andmaximum effective strain are located in the regions of the titanium sheet close to the entryradius of the die. By contrast, Fig. 3(c) shows that the maximum effective stress is distributeduniformly over the entire surface of the ellip-cylindrical product. Fig. 4 shows the general product appearance, the damage distribution, the effective straindistribution and the effective stress distribution following superplastic blow-forming underconditions of: t = 1.5 mm, a = 40 mm, b = 20 mm, R = 7 mm, r = 2 mm, h = 10 mm, m = 0.5,T = 1000°C, and a strain rate of 0.1 s-1. The results reveal that under these modifiedprocessing conditions, the maximum damage and effective strain are induced near the rootradius of the die (see Figs. 4(a) and 4(b), respectively). However, the maximum effectivestress is once again distributed uniformly over the entire surface of the blow-formed product. Fig. 5 illustrates the variation of the titanium alloy thickness following blow-formingunder conditions of t = 1.5 mm, a = 40 mm, b = 30 mm, R = 5mm, r = 2 mm, h = 9 mm, m =0.5, T = 1000°C, and a strain rate of 0.1 s-1. As shown, the maximum sheet thickness (1.42 ~1.46 mm) occurs near the entry radius region of the die, while the minimum sheet thickness(0.68 ~ 1.02 mm) occurs near the root radius region of the die. Fig. 6 presents a mesh model showing the fracture of the titanium alloy sheet followingblow-forming under conditions of t =1.5 mm, a = 40 mm, b = 30 mm, R = 5 mm, r = 2 mm, h= 10 mm, m = 0.2, T = 1000°C, and a strain rate of 0.1 s-1. The results indicate that underthese particular blow-forming conditions, the flow stress induced within the titanium sheetexceeds the yield strength of the titanium alloy and causes the alloy to fracture. Table III summarizes the thickness of the titanium alloy sheet at various positions of theellip-cylindrical product following blow-forming under each of the 21 conditions given inTable II. As shown, both the initial pressure and the pressure increase applied after 5 steps inthe simulation process are assigned values of 1 MPa, 1.5 MPa or 2 MPa. Overall, the resultsreveal that the thickness of the titanium sheet varies in the range 1.22 ~ 1.37 mm in thelong-axis region of the entry radius part of the die, 0.49 ~ 0.96 mm in the long-axis region ofthe root radius part of the die, 0.71 ~ 1.30 mm in the short-axis region of the entry radius partof the die, and 0.47 ~ 1.21 mm in the central region of the die. In other words, the resultsconfirm that the minimum thickness of the ellip-cylindrical product occurs in the regionclosest to the die root radius. 22
7.
Chen, Chen, Lin, Jheng, Chen: Finite Element Analysis of Superplastic Blow-Forming of …t = 1.5 mm, a = 40 mm, b = 30 mm, R = 5 mm, r = 2 mm, h = 9 mm, m = 0.5, T = 1000°C,Strain rate = 0.1 s-1 Max. 0.769 (a) Damage 0.496 (b) Effective strain 42.7 MPa (c) Effective stressFigure 3: Distribution of damage, effective strain and effective stress in blow-formed Ti-6Al-4V ellip-cylindrical product (one-quarter die). 23
8.
Chen, Chen, Lin, Jheng, Chen: Finite Element Analysis of Superplastic Blow-Forming of …t = 1.5 mm, a = 40 mm, b = 20 mm, R = 7 mm, r = 2 mm, h = 10 mm, m = 0.5, T = 1000°C,Strain rate = 0.1 s-1 (a) Appearance of productMax. 1.32 (b) Damage1.02 mm/mm (c) Effective strain43.1 MPa (d) Effective stressFigure 4: Appearance and distributions of damage, effective strain and effective stress in blow-formed Ti-6Al-4V ellip-cylindrical product (full die). 24
9.
Chen, Chen, Lin, Jheng, Chen: Finite Element Analysis of Superplastic Blow-Forming of …t = 1.5 mm, a = 40 mm, b = 30 mm, R = 5 mm, r = 2 mm, h = 9 mm, m = 0.5, T = 1000°C,Strain rate = 0.1 s-1 1.46 1.321.42 1.15 1.18 1.13 0.68 1.02 1.16 1.14 1.21Figure 5: Distribution of ellip-cylindrical product thickness (units: mm).t = 1.5 mm, a = 40 mm, b = 30 mm, R = 5 mm, r = 2 mm, h = 10 mm, m = 0.2, T = 1000°C,Strain rate = 0.1 s-1 Fracture voidFigure 6: Fracture of ellip-cylindrical product.4. CONCLUSIONSThis study has utilized DEFORMTM 3D FE software to investigate the plastic deformationbehaviour of Ti-6Al-4V titanium alloy during its superplastic blow-forming into a closedellip-cylindrical die. The simulations focus principally on the respective effects of the shearfriction factor, the die entry radius, the die height and the length of the die’s short axis on thethickness, effective stress, effective strain and critical damage characteristics of the formedsheet. The simulation results support the following major conclusions: (1) the maximumeffective stress is distributed uniformly over the entire surface of the ellip-cylindrical product;(2) the minimum sheet thickness is induced in the region of the ellip-cylindrical product closeto the root radius region of the die; and (3) in the event that the flow stress induced within theblow-forming process exceeds the yield strength of the Ti-6Al-4V alloy, the ellip-cylindricalproduct fractures in the flat base region. Overall, the simulation results confirm the suitabilityof the FE software for modelling the superplastic blow-forming of Ti-6Al-4V titanium alloy. 25
10.
Chen, Chen, Lin, Jheng, Chen: Finite Element Analysis of Superplastic Blow-Forming of … Table III: Summary of ellip-cylindrical product thickness for all considered simulation conditions. Factors Increasing Thickness Thickness Thickness Initial Thickness of pressure of die entry of die root of die entry Pressure central after 5 steps radius (mm) radius (mm) radius (mm) No. (MPa) position (mm) (MPa) (long axis) (long axis) (short axis) 1 2 2 1.32 0.64 0.95 0.82 2 2 2 1.30 0.57 0.82 1.00 3 2 2 1.32 0.75 0.71 0.93 4 2 2 1.26 0.50 1.17 0.92 5 2 2 1.27 0.57 1.06 0.88 6 2 2 1.27 0.65 0.98 0.87 7 2 2 1.25 0.84 0.98 1.07 8 2 2 1.25 0.76 1.05 0.68 9 2 2 1.30 0.96 0.88 0.48 10 2 2 1.23 0.78 1.05 0.47 11 2 2 1.22 0.76 1.04 0.69 12 2 2 1.30 0.89 0.99 0.63 13 2 2 1.35 0.56 1.11 1.08 14 1.5 1.5 1.34 0.56 1.30 1.07 15 1.5 1.5 1.37 0.51 1.19 1.02 16 1 1 1.22 0.49 1.24 1.16 17 1 1 1.28 0.57 1.25 1.15 18 1 1 1.29 0.61 1.21 1.03 19 1.5 1.5 1.32 0.68 1.15 1.21 20 1.5 1.5 1.34 0.72 1.20 1.19 21 1.5 1.5 1.37 0.79 1.21 1.03REFERENCES[1] Miller, Q. S.; White, J. (1988). Chapter in: Superplasticity in Aerospace, Heikkenen, H. C.; McNelley, T. R. (Eds.), AIME, Warrendate, PA, Vol. 211[2] Al-Naib, T. Y. M.; Duncan, J. L. (1970). Superplastic metal forming, International Journal of Mechanical Sciences, Vol. 12, 463-477[3] Hwang, Y. M.; Lay, H. S.; Huang, J. C. (2002). Study on superplastic blow-forming of 8090 Al-Li sheets in an ellip-cylindrical closed-die, International Journal of Machine Tools & Manufacture, Vol. 42, 1363-1372[4] Hwang, Y. M.; Lay, H. S. (2003). Study on superplastic blow-forming in a rectangular closed-die, Journal of Materials Processing Technology, Vol. 140, 426-431[5] Senthil Kumar, V. S.; Viswanathan, D.; Natarajan, S. (2006). Theoretical prediction and FEM analysis of superplastic forming of AA7475 aluminum alloy in a hemispherical die, Journal of Materials Processing Technology, Vol. 173, 247-251[6] Morsy, A. W. E.; Manabe, K. I. (2002). FE simulation of rectangular box forming using material characteristics from the multi-dome forming test, Journal of Materials Processing Technology, Vol. 125-126, 772-777 26
11.
Chen, Chen, Lin, Jheng, Chen: Finite Element Analysis of Superplastic Blow-Forming of …[7] Hwang, Y. M.; Yang, J. S.; Chen, T. R.; Huang, J. C.; Wu, W. U. (1998). Analysis of superplastic blow-forming in a conical closed die, International Journal of Mechanical Sciences, Vol. 40, No. 9, 867-885[8] Bonet, J.; Wood, R. D.; Collins, R. (1994). Pressure-control algorithms for the numerical simulation of superplastic forming, International Journal of Mechanical Sciences, Vol. 36, No. 4, 297-309[9] Kim, Y. H.; Lee, J. M.; Hong, S. S. (2001). Optimal design of superplastic forming processes, Journal of Materials Processing Technology, Vol. 112, 166-173[10] Huang, A.; Lowe, A.; Cardew-Hall, M. J. (2001). Experimental validation of sheet thickness optimization for superplastic forming of engineering structures, Journal of Materials Processing Technology, Vol. 112, 136-143[11] Yarlagadda, P. K. D. V.; Gudimetla, P.; Adam, C. (2002). Finite element analysis of high strain rate superplastic forming (SPF) of Al-Ti alloys, Journal of Materials Processing Technology, Vol. 130-131, 469-476[12] Hambli, R.; Potiron, A.; Guerin, F.; Dumon, B. (2001). Numerical pressure prediction algorithm of superplastic forming processes using 2D and 3D models, Journal of Materials Processing Technology, Vol. 112, 83-90[13] Verma, R.; Kim, S. (2007). Superplastic behavior of copper-modified 5083 aluminum alloy, Journal of Materials Engineering and performance, Vol. 16, 185-191[14] Nazzal, M. A.; Khraisheh, M. K.; Darras, B. M. (2004). Finite element modeling and optimization of superplastic forming using variable strain rate approach, Journal of Materials Engineering and performance, Vol. 13, 691-699[15] Wu, H. Y.; Perng, J. Y.; Shis, S. H.; Chiu, C. H.; Lee, S.; Wang, J. Y. (2006). Cavitation characteristics of a superplastic 5083 Al alloy during gas blow forming, Journal of Materials Science, Vol. 41, 7446-7453[16] Sorgente, D.; Scintilla L. D.; Palumbo, G.; Tricarico, L. (2010). Blow forming of AZ31 magnesium alloy at elevated temperatures, International Journal of Material Forming, Vol. 3, No. 1, 13-19[17] Chen, D. C.; Lin, J. Y.; Jheng, M. W.; Chen, J. M. (2007). Design of titanium alloy superplastic blow-forming in ellip-cylindrical die using Taguchi method, Proceedings of the 35th International MATADOR Conference, Taipei, Taiwan, 105-109[18] Chen, D. C.; Wang, H. N. (2008). A finite element analysis of the superplastic blow-forming in an awl-shaped die with titanium alloy, Computer Methods in Materials Science, Vol. 8, No. 3, 130-137[19] Kim, Y. J.; Yang, D. Y. (1985). A formulation for rigid-plastic finite element method considering work-hardening effect, International Journal of Mechanical Sciences, Vol. 27, No. 7-8, 487-495[20] Klocke, F.; Breuer, D.; Raedt, H. (2002). Prediction of Ductile Fracture in Cold Forming Processes, Proceedings of the 7th ICTP, Advanced Technology of Plasticity, Yokohama, Japan, Vol. 1, 721-726 27
Be the first to comment